solving raw materials challenges
Click here to load reader
Post on 16-Apr-2015
Embed Size (px)
SOLVING RAW MATERIAL CHALLENGESBy Linda M. Hills, Senior Scientist; Vagn Johansen, Senior Principal Scientist; and F. MacGregor Miller, Senior Principal Scientist Construction Technology Laboratories, Inc.
Abstract A comprehensive understanding of the chemical and physical aspects of raw material transformation into clinker is an important foundation to increasing production, reducing costs, and improving quality at the cement plant. Clinker formation relies on numerous kiln feed properties and pyroprocessing conditions. Understanding the influential properties of the feed (chemistry, fineness, uniformity, and mineralogy) can lead to improvements in its burnability and therefore in the efficiency of plant operations. The paper discusses clinker formation, its relation to kiln feed properties, and the importance of optimizing burnability by careful mix control, good mix homogeneity, and tailoring the burning process to the raw mix. The burnability and kiln feed are discussed in relation to specific fuel consumption. When the raw materials available make it hard to achieve burnability goals, the use of fluxes and/or mineralizers may be helpful. Fluxes and mineralizers indirectly affect burnability by promoting clinker phase formation to occur earlier; their effect on clinker formation and cement quality is briefly described. Fluoride-containing compounds have proven to be the most effective mineralizers in cement clinkering reactions. However, an excessive amount of fluoride may delay cement setting time. Emphasis is placed on the effects of changes in raw material burnability and clinker formation on kiln operations, finish mill productivity, and the properties of the resulting cement. Introduction Plant management is constantly under pressure to maintain or increase production rates and reduce costs, without sacrificing quality. These three are challenging goals, especially achieving all three simultaneously. Understanding the process of clinker manufacture - how raw materials are transformed into clinker - is the key. This transformation involves both chemical and physical processes. The microstructure of clinker is a function of kiln feed properties and the pyroprocessing conditions. Knowing what happens where, why, and how, can lead to optimizing production, costs, and quality. In turn, the clinker microstructure and composition directly affect how the phases hydrate and contribute to cement performance in fresh and hardened concrete. Given its relationship to both efficiency of plant operations and cement performance, the importance of clinker formation cannot be overestimated. Clinker Formation Stated simply, the chemical aspect of clinker formation is the combination of silica with calcium to produce hydraulic compounds. However, the actual transformation of the raw materials into clinker involves a combination of chemical and physical processes as the material passes through the kiln system. The general process of clinker formation is described in Figure 1. The transformation concludes with the primary clinker phases: Alite: impure tricalcium silicate, generally termed C3S Belite: impure dicalcium silicate, normally termed C2S Aluminate: tricalcium aluminate, C3A Ferrite: nominally tetracalcium aluminoferrite, C4AF
Figure 1. A simplified view of the clinkering reactions in a Portland cement kiln (Hills 2000)
To 700C Water is lost from clay minerals. Dehydrated clay recrystallizes. Some reactive silica may displace CO2 from CaCO3. H 20
Clay particle Limestone particle
700-900C As calcination continues, free lime increases. Calcination maintains feed temperature at around 850C. Lower-limed aluminate and ferrite form.
900-1150C Reactive silica combines with CaO to begin stages of C2S formation. 1150-1200C When calcination is complete, temperature increases rapidly. Small belite crystals form from combination of silicates and CaO.
Round belite crystals 1200-1350C Above 1250C, liquid phase is formed. Belite and free CaO form alite in the liquid.
Angular alite crystals 1350-1450C Belite crystals decrease in number, increase in size. Alite crystals increase in size and number.
Cooling Upon cooling, the C3A and C4AF crystallize from the liquid phase. Lamellar structure appears in belite crystals.
Figure 2. Clinker silicate phases as observed under a microscope (polished section with nital etch) Alite (C3S) normally hexagonal crystals observed in cross-section, 25-50m in length.
Belite (C2S) normally 25-40m rounded crystals with multidirectional lamellae.
Figure 3. Phases in clinker interstitial (polished section with nital etch) Tricalcium aluminate (C3A): Observed in etched and polished clinker as blue to gray angular crystals in the interstitial. High alumina ratio will produce greater amount of aluminate than ferrite.
Ferrite (C4AF) appears more reflective than C3A in an etched polished surface
Figure 4. Clinker photomicrograph demonstrates reaction between belite and free CaO to form alite (polished section with nital etch) Free CaO crystals Either properties of the raw materials, mix homogeneity, or the pyroprocessing conditions did not allow the complete transformation to alite to take place.
Improving Pyroprocessing Efficiency The amount of energy needed to form clinker depends on various properties of the raw materials. Using a burnability equation such as that shown below can identify the specific factors that influence burnability at a particular plant, and provide the information needed to make appropriate improvements. This approach can also be used to anticipate changes caused by the introduction of new raw materials. Replacing raw materials with others because they are less expensive, or to correct the chemical composition may change how difficult it is to burn the new kiln feed. Raw Material Properties and Burnability The raw materials used are designed and proportioned to provide the appropriate amounts of the various clinker phases. Specific properties of the materials are critical to plant efficiency and energy consumption, based on their burnability. Burnability is the ease with which the raw materials are transformed into the desired clinker phases, and is commonly measured by the amount of free (un-reacted) lime remaining in the clinker (low free lime indicates an easy-to-burn mix). Ordinarily, the burnability is a measure of the ease of formation of alite from belite and free lime, as formation of the other phases is normally much easier to achieve. The lower the temperature at which the targeted free lime can be obtained, the better is the burnability of the kiln feed. The burnability of a raw mix is determined by its chemical composition, the mineralogy of its component materials, and its fineness. There are a number of equations that relate the burnability of a feed to the composition and fineness of the minerals (Fundal 1979, Petersen and Johansen 1979, Christensen 1979, Ludwig 1973). One example is the burnability equation developed at F. L. Smidth (Theisen 1992), provided below. The importance of a burnability equation is not to provide an exact value of the free lime of clinker made from a given raw mixture; it is more important that it gives insight into the effect of raw material properties on the resulting free lime (clinker burnability) on a relative basis. CaO1400C =[ 0.343(LSF-93) + 2.74(SR-2.3)] + [0.83Q45 + 0.10C125 +0.39R45] Where: CaO1400C = is the free lime after burning for 30 minutes at 1400oC LSF = %CaO/(2.8%SiO2+1.18%Al2O3+0.65%Fe2O3) SR = % SiO2/(% Al2O3+% Fe2O3) Q45 = % quartz grains coarser than 45m C125 = % calcite grains coarser than 125m R45 = % other acid-insoluble minerals, (e.g. feldspar) coarser than 45m The first part of the equation (first bracket) represents contribution from the chemical properties of the raw mix. The LSF (lime saturation factor) represents the CaO of the mix, while the SR (silica ratio or modulus) is related to the amount of liquid phase at the burning zone temperature. Decreasing the SR is equivalent to increasing the amount of liquid phase; since the liquid is the transport medium for the reactants, more liquid can transport more reactants during a given time and therefore, the burnability is improved. Note the relative magnitude of the coefficients for LSF and SR; the role of the liquid for the clinker reactions is important, not only for the chemical reactions but also for the formation of clinker nodules (the physical aspect of clinker formation). The second part of the burnability equation (second bracket) represents the contribution to the burnability from the mineralogy and fineness of the raw mix. The percentages of coarse particles represented by C125, Q45, and R45 are determined by the overall fineness of the raw mix on the one hand, and the mineralogical properties of the raw materials on the other. Differences in the mineralogy of the mix components leads to differences in grindability, which in turn will result in variations in the chemical composition of the different size fractions of the raw mix. For example, since quartz is hard to grind, the SiO2 content of the coarser fraction of the mix will normally be higher than that of the finer fraction. Note
that the quartz fineness is more significant than fineness of other materials, as indicated by its larger coefficient in the equation. The equation provides a virtual burnability test to analyze the factors affecting burnability and free lime of the clinker. There is a relation between the free lime determined by the virtual burnability test and the free lime of the clinker. Although not identical, it can be assumed that the virtual burnability free lime will correspond to a certain constant clinker free lime for a given constant kiln operation. Further, for a given kiln and set of raw materials, if the virtual burnability free lime of the kiln feed changes and the kiln process parameters remain the same, the clinker free lime will change in a way so the ratio between the virtual free lime value and the clinker free lime remains the same as before the change. For instance if the virtual free lime is 3.2 % and the average clinker free lime is 1.4 % for a given steady state of kiln operation, the ratio is 2.3. This defines a burning index and is a measure for how the kiln in that state of operation on average burns the kiln feed. Reasons for variations in burnability could be insufficient raw mix control and/or homogenization of the kiln feed. The resulting clinker will vary in free lime content, and the normal reaction from kiln operators is to burn harder and eventually operate the kiln on the hot side to avoid large variations in the clinker free lime. One penalty that results is increased specific fuel consumption. An example of the relation between the burnability index and the specific fuel consumption is the result of analysis of data from a 2000 mtpd kiln with planetary coolers, as shown in Figure 5. Based on averages of kiln feed chemical composition and fineness, the virtual burnability free lime was determined and together with the average clinker free lime for the same period, the burning index ratio calculated.
3.5 3.4 3.3Fuel Consumption (MMbtu/ton)
3.2 3.1 3.0 2.9 1.5 2 2.5 3 3.5
Burning Index Ratio (virtual burnability/clinker free lime) Figure 5. Burning Index Ratio (virtual burnability free lime/clinker free lime) Each point represents the average over a 4-week period. No corrections were made for kiln downtime during the 4week periods, which might explain the outliers.
An increasing burnability index means harder burning, resulting in higher specific fuel consumption. Figure 5 can be used to analyze the effect of kiln feed homogeneity on the specific fuel consumption. As an example, consider a kiln with average feed composition corresponding to LSF = 98 % and silica ratio, SR = 2.8 (corresponding to about 66% C3S), with virtual burnability free lime of 3.2% and an average clinker free lime 1.4%. For a steady state kiln operation and a constant homogeneous kiln feed, the burning index is 3.2/1.4=2.3. In reality the kiln feed composition will vary between certain limits. In the first example, assume the variations in LSF and SR are +/- 0.6% and +/- 0.07 respectively. Using the equation for the virtual burnability test given above, these variations correspond to a variation of the virtual burnability test free lime between 3.8 and 2.6%. For the steady state kiln operation referred to
above, with burning index = 2.3, this will result in clinker free lime between 1.7 and 1.1%. In the second example let the kiln feed composition vary +/- 2% in LSF and +/- 0.23 in SR. This corresponds to variations in the virtual burnability free lime between 4.5 and 1.9%, and for constant kiln operation a variation of the clinker free lime between 2.0% and 0.8%. As a result of the less homogenous kiln feed in the last example, the clinker free lime will vary within wider limits. If the operation is changed to harder burning in order to bring the maximum clinker free lime down to the average value and narrow the variation in free lime, the burning index will change from the original 2.3 to 4.5/1.4=3.2. From Figure 5 such a change corresponds to an increase of about 6% in specific fuel consumption. Once again, an understanding of burnability and free lime content is important. There is a relation between the virtual burnability free lime and the free lime of the clinker from the kiln. This burning index ratio can be used as a process parameter. If the kiln is operated in steady state, the ratio is constant. However, if the virtual burnability deteriorates (i.e. decrease in mix fineness or change in chemistry), and the kiln is kept in the same steady state, then the clinker free lime will increase. The usual operator reaction to an increase in clinker free lime is to burn harder. However, if an examination of the kiln feed were performed to identify the cause for the increase in virtual burnability free lime, the corresponding increase in clinker free lime would be anticipated. The kiln operators would therefore know what to expect, and would not necessarily constantly operate the kiln on the hot side. The examples given above also emphasize the importance of good raw mix control and kiln feed homogenization vis--vis the specific fuel consumption. Most often, the mineralogy and fineness change little compared to the chemical composition unless the raw material sources are changed. Therefore, using the chemical contribution portion of the burnability equation is helpful. This calculation will give an indication of feed burnability very quickly. An example of chemical analysis and calculation of its contribution to burnability is below. Note that the trend in burnability is more easily detected when looking at the calculated chemical contribution instead of the individual factors of LSF and SR alone. LSF 95.2 95.6 94.9 95.9 95.8 SR 2.2 2.3 2.8 3.1 3.2 Chemical contribution [0.343(LSF-93) + 2.74(SR-2.3)] 0.48 0.89 2.02 3.19 3.43
Fluxes and Mineralizers The use of fluxes and mineralizers can promote clinker phase formation, and therefore improve efficiency of the pyroprocessing system. By definition, a flux promotes a reaction by increasing the amount of liquid at a given temperature; for example, Al2O3 and Fe2O3 are fluxes for the formation of alite. A mineralizer promotes the formation of a particular solid phase through its incorporation in one or more of the solid phases (normally either alite or belite). A general view demonstrating the process of clinker formation using a flux or mineralizer, contrasted with using neither is outlined in Figure 6.
Figure 6. Simplified clinkering reactions in a Portland cement kiln with no additions, with mineralizer, and with flux.
Clinkering with mineralizer
Clinkering with flux
Liquid phase formation occurs earlier (at lower temperature).
Mineralizers promote earlier silicate phase formation (some enhance liquid formation, some form intermediate phases).
Increased liquid phase allows more C3S (alite) to form.
Without mineralizer or flux, clinker phases are still forming in kiln.
With mineralizers and fluxes, desired clinker phases are formed earlier, and is discharged from kiln. The result: residence time in kiln is reduced, and less energy is required.
Fluxes and mineralizers have been studied in laboratory experiments and in practice (Flint 1939, Johansen and Christensen 1979, Surana and Joshi 1990, Erhard 1994, Altun 1999). A series of different compounds have been used; however, the ones with the most practical application are fluorides. Fluoride-containing mineralizers have been used since the late 1800s (Bhatty 1996). Fluoride-containing compounds such as CaF2, NaF, BaF2, and MgF2, are all effective primarily as mineralizers, although CaF2 has enjoyed the greatest use. Alkali- and alkaline-earth fluorosilicate salts like Na2SiF6 and MgSiF6 can also achieve similar mineralizing effects (Lea 1971). The effect of 5 to 10% fluorspar on the clinkering of two cement compositions was reported (Klemm 1976) and as expected, these massive additions resulted in both a reduction in clinkering temperature and a consequent retardation of cement setting. However, there was little effect on the 28-day strength of hydrated cements. Although fluoride-containing compounds have been proven to be the most effective mineralizer in cement clinkering reactions, a number of other possible fluxes and mineralizers have been studied. These have included gypsum and sulfate mineral tailings, fluoro-gypsum, phosphorus-containing calcareous tailings in combination with gypsum/fluorspar and others; all showed some effect either as fluxes or mineralizers but the studies did not result in practical use. The benefits of added fluoride in achieving desired free lime levels at lower temperatures are illustrated by a study in which the same rather hard-burning raw mix was burned with and without the addition of 0.25% fluoride. In this particular case, the fluoride was added as a fluoride salt. The mixes were burned at 1450C (2640F) for 60 minutes. The resulting free lime content of the control clinker was 5.05%, while that of the clinker to which fluoride was added was 2.31%. A further demonstration of the benefits to burnability of added fluoride was carried out using the so-called sandwich technique. In this technique, two compacts are prepared. The first is calculated to be an alite/free lime mixture, while the second is calculated to be an alite/belite mixture after clinkering. The compacts had the compositions shown in the table below. Reagent Calcium carbonate Quartz (SiO2) Alumina (Al2O3) Ferric Oxide (Fe2O3) Magnesium Hydroxide Sodium Carbonate (Na2CO3) Potassium Carbonate (K2CO3) High Lime Compact, % 78.9 10.73 3.86 1.93 3.05 0.51 1.02 Low Lime Compact, % 74.3 15.33 3.86 1.93 3.05 0.51 1.02 Alite Belite